**4.3 Application 1 - Data from Ogi et al., 2002**

**4.3.2 Results and discussion**

, (4.23a)

m_{2} = log
C_{44}

50

. (4.23b)

We then constructed a weakly informative prior by choosing the covariance matrix to be 0.1 times the 2-by-2 identity matrix I2, which gives a broad distribution in the stiffness space (Fig.4.2).

For the pairing, we considered the M = 50 first predicted frequencies, letting
room for up to k_{max} = 8 potentially non-observed frequencies. The expectation
λ was set to 1. It gave equally high prior probability (≈ 0.37) of having missed
k= 0andk= 1resonant frequencies and a decreasing probability for largerk, thus
reflecting our prior knowledge that the frequencies are easily measured on a very
low damping material.

We used the noninformative prior p(σ^{2}) = 1/σ^{2} for the variance. We set an
upper boundary of σ^{2} <0.03^{2}, corresponding to a misfit of 3% between predicted
and measured frequencies, much larger that what can be expected from a successful
RUS experiment.

4.3.2 Results and discussion

The 8 starting points generated from the procedure described in Section 4.2.3.4are
located by crosses in Fig. 4.2. We see that the 8 starting values of C_{44} are close.

This is due to the fact that the first predicted mode is usually an almost pure shear
mode, depending mainly on C44. Since this mode is always paired with the first
measured frequency, it has the effect of almost fixing the shear coefficient C_{44} close
to the correct value. The coefficientC11 remains largely undetermined at this step.

C11(GPa) C 44(GPa)

0 200 400 600 800 1000

0 50 100 150 200

Figure 4.2: Application 1: prior probability in the space of the stiffness coefficients corresponding to the bivariate normal prior distribution onm, centered onm1andm2

with covariance equal to0.1×I_{2}. The contour lines enclose respectively 10, 68, 95, 99,
and 99.99 % of the distribution. The crosses locate the randomly generated starting
points of the 8 Gibbs chains.

20 40 60 80 100

100 150 200 250 300 350 400 450

Gibbs sampler iteration C 11(GPa)

40 50 60 70 80 90 100

106 108 110 112

Figure 4.3: Application 1: sampled values of C11 for the 100 first iterations of the 8 Gibbs chain. After 40 iterations, all the chains have converged to the same location.

4.3. Application 1 - Data from Ogi et al., 2002 79

104 106 108 110 112 114
C_{11}(GPa)

26.55 26.6 26.75 26.85

C44(GPa)

1 2 3 4 5

σ(x10^{−3})

Figure 4.4: Application 1: Histograms of the stiffness coefficients and error term σ obtained from Gibbs sampling using the frequency data of the alluminium alloy specimen fromOgi et al.(2002).

Convergence of the 8 parallel chains was observed at the first convergence test, after 100 iterations of the Gibbs sampler, but we let them run for 900 more iterations (∼ 4 min of computation time). The convergence was indeed reached after about 40 iterations, as it can be seen on Fig. 4.3. After discarding the 100 first samples, chains were pooled and the sampled m transformed back to stiffness coefficients to evaluate the posterior distribution. Any other elastic modulus (e.g. Young’s modulus or Poisson’s ratio) could also have been calculated.

The histograms for C11,C44, and σ are plotted on Fig. 4.4. It can be observed that the marginal posterior distributions of the stiffness constants have a normal shape while the marginal for σ is asymmetric. The posterior means and standard deviations forC11,C44 were respectively taken as the estimate of the stiffness con-stant and uncertainties. Forσ, the point of maximum marginal posterior probability was estimated from the histogram. The results are given in Table4.1, and compared to the estimates obtained assuming the exact pairing. These estimates were obtained from the quasi-Newton method described in section 4.2.3.2. In that case the esti-mated standard deviation is the relative root-means-square error between measured and predicted frequencies at the end of the fit. The result obtained with uncertain and exact pairing are almost identical and the uncertainties are only slightly larger in the first case, which shows that the approach proposed here produces results that are almost as accurate and precise as the results obtained using the exact pairing deduced from laser measurements. We also recall the values obtained byOgi et al.

using more than 80 frequencies with exact pairing (only the 42 first frequencies were given in the paper). The values are slightly different but agree with the uncertainty intervals.

The 42 published frequencies correspond to the actual 42 first resonant modes of the specimen (no missed frequencies). Our algorithm correctly and unambiguously identified that no frequency was missed, i.e. we obtainedp(k = 0) = 1. Moreover,

Table 4.1: Application 1: parameters estimated from the proposed Gibbs sampling method for the data fromOgi et al.(2002), compared to estimations knowing the exact pairing of the frequencies.

Gibbs Exact pairing Ogi et al. (2002)

Nb freq. 42 42 >80

C11 (GPa) 108.8±0.9 109.0±0.7 109.26 C44 (GPa) 26.68 ±0.03 26.68 ±0.02 26.72

Variance (%) 0.24 0.23 0.2

since the exact pairing is known we can compare the pairings obtained through Gibbs sampling to the correct pairing. In Table 4.2, the sampled group symmetry labels for each mode are listed against the exact label obtained from Laser interferometry.

We can see that 18 out of 42 modes are uniquely paired and that a total of 32 modes are confidently identified (>95%probability) with the correct predicted mode. The other modes are identified with larger uncertainties and with up to 4 possibilities of pairing. However, the most probable mode label is always the correct one, except for two pairs of modes that were inverted (modes 38−39 and 41−42). All cases of uncertain or inexact identifications correspond to resonant frequencies that are very close to each others, compared to the estimated standard deviation of the experimental frequencies (0.24%). It is then not surprising that these frequencies cannot be confidently paired to a unique predicted frequency. But we argue that it is precisely in those cases that the exact pairing matters the less. Indeed, inverting two or more frequencies that are separated by less than the standard deviation can only have a negligible influence on the estimated stiffness.

The correct pairing was obtained by the method (except for some very close modes) using only the frequencies, which shows that the information on the vibration modes is indeed contained in the distribution of the frequencies. Then, getting the modal shapes experimentally only provides redundant information here.

Table 4.2: Application 1: experimental resonant frequencies and group symmetry label from Laser-based RUS measurement (Ogi et al.,2002) and group symmetry labels proposed during Gibbs sampling with their percentage of occurrence. Labels indicate belongings to one of the 8 distinct symmetry groups and the ordering in each group, following the notation introduced byMochizuki (1987)

f_{exp} (kHz) Mode Modes Gibbs (%of occurrence)

116.716 A_{u}-1 A_{u}-1 (100) - -

-143.783 A_{u}-2 A_{u}-2 (100) - -

-158.081 B1u-1 B1u-1 (100) - -

-Continued on next page

4.3. Application 1 - Data from Ogi et al., 2002 81

Table 4.2 : Continued from previous page fexp (kHz) Mode Modes Gibbs (%of occurrence)

166.500 B2u-1 B2u-1 (100) - -

-169.523 B_{1g}-1 B_{1g}-1 (100) - -

-177.846 B2g-1 B2g-1 (100) - -

-183.875 B3u-1 B3u-1 (99.2) B3g-1 (0.8) -
-186.047 B_{3g}-1 B_{3g}-1 (99.2) B_{3u}-1 (0.8) -

-190.341 Ag-1 Ag-1 (100) - -

-197.386 B_{1u}-2 B_{1u}-2 (100) - -

-201.136 A_{g}-2 A_{g}-2 (100) - -

-207.386 B3g-2 B3g-2 (100) - -

-209.836 A_{g}-3 A_{g}-3 (100) - -

-214.753 B_{2g}-2 B_{2g}-2 (100) - -

-223.548 B3u-2 B3u-2 (100) - -

-231.266 B_{2u}-2 B_{2u}-2 (100) - -

-233.538 B3g-3 B3g-3 (99.1) B1g-2 (0.9) -
-234.717 B1g-2 B1g-2 (99.1) B3g-3 (0.9) -
-250.980 A_{g}-4 A_{g}-4 (55.0) A_{u}-3 (44.7) B_{2g}-3 (0.3)
-251.256 Au-3 Au-3 (54.6) Ag-4 (44.7) B2g-3 (0.7)
-252.742 B_{2g}-3 B_{2g}-3 (99.0) A_{u}-3 (0.7) A_{g}-4 (0.3)
-256.122 B_{1u}-3 B_{1u}-3 (98.4) B_{3u}-3 (1.5) A_{g}-5 (0.1) B_{2u}-3 (0.0)
257.595 B3u-3 B3u-3 (72.6) Ag-5 (19.6) B2u-3 (6.3) B1u-3 (1.5)
258.118 A_{g}-5 A_{g}-5 (51.0) B_{2u}-3 (25.9) B_{3u}-3 (23.0) B_{1u}-3 (0.1)
259.035 B2u-3 B2u-3 (67.9) Ag-5 (29.3) B3u-3 (2.8)

-268.540 B1g-3 B1g-3 (100) - -

-277.113 B_{2u}-4 B_{2u}-4 (99.9) B_{3u}-4 (0.1) -
-278.762 B3u-4 B3u-4 (99.9) B2u-4 (0.1) -

-282.311 B_{1u}-4 B_{1u}-4 (100) - -

-293.686 B_{3u}-5 B_{3u}-5 (100) - -

-304.159 B2u-5 B2u-5 (58.9) B1u-5 (41.1) -
-304.464 B_{1u}-5 B_{1u}-5 (58.9) B_{2u}-5 (41.1) -

-310.109 B1u-6 B1u-6 (100) - -

-316.197 B1g-4 B1g-4 (97.7) B2g-4 (2.3) -
-317.392 B_{2g}-4 B_{2g}-4 (97.7) B_{1g}-4 (2.3) -
-326.462 Au-4 Au-4 (100) B3g-4 (0.0) -
-329.034 B_{3g}-4 B_{3g}-4 (100) A_{u}-4 (0.0) -
-332.441 A_{g}-6 B_{2u}-6 (70.9) A_{g}-6 (29.1) -
-333.364 B2u-6 Ag-6 (70.9) B2u-6 (29.1) -
-336.650 B_{1g}-5 B_{1g}-5 (69.6) A_{g}-7 (18.8) B_{2g}-5 (11.6)

-Continued on next page

Table 4.2 : Continued from previous page fexp (kHz) Mode Modes Gibbs (%of occurrence)

337.359 B2g-5 Ag-7 (38.1) B2g-5 (36.7) B1g-5 (25.1)
-338.276 A_{g}-7 B_{2g}-5 (51.7) A_{g}-7 (43.1) B_{1g}-5 (5.2)